Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4852
Fabrication and Testing Of Composite Powder Materials
from Tamarind Seeds and Palm Date Seeds Using Epoxy
Mr. Pediredla Sudhir Kumar &
Mr. T.Naresh Kumar
1 PG Scholar, Department of MECH,Mallareddy Engineering College (AU), main campus, maisammaguda,
Hyderabad, Telangana, INDIA, PIN-500100 E-Mail Id: firstname.lastname@example.org
2 Assistant Professor, Department of MECH,Mallareddy Engineering College (AU), main campus, maisammaguda,
Hyderabad, Telangana, INDIA, PIN-500100 E-Mail Id: email@example.com Abstract:
Dates from date palm (Phoenix dactylifera) trees are popular for providing a staple food for millions of
people around the world, and tamarind
(TamerindusIndica) is the other product which is used as food ingredient as pulp tamarind. Here we will use both tamarind and dates seed powders as the composite material, which are mostly treated as waste in our day to day life. As the composite material consists of matrix and reinforcement, in this the particulates tamarind and dates seed powders are used as reinforcement and matrix used is Araldite Standard Epoxy resin AW106 along with hardener HV953. The reinforcement used is tamarind dates seed powders are mixed with the matrix taken in the fixed ratios, with different proportions. Then the composite is fabricated and tested for strength and hardness. The tests performed are impact and Rockwell hardness test. Different compositions of the matrix and epoxy is fabricated and compared among composites prepared and result is shown. Composite materials are substitute for the conventional plastics and possess higher mechanical properties then those materials.
Definition and characteristics:
Composite materials can be characterized as the blend of various materials manufactured together frame a one of a kind material, every material hold
their unique mechanical, substance properties. A basic composite is a material framework comprising of at least two stages on tiny scale, one of the stage is generally spasmodic, stiffer and more grounded and is called fortification while less solid and weaker stage is ceaseless for the most part in fluid shape is called Matrix.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4853
composites, the typically constant fiber support is the foundation of the material that decides its firmness and quality toward the filaments. The network stage gives assurance to the fiber. In this undertaking the tamarind seeds and the Palm date seeds powders goes about as the filaments and epoxy pitch goes about as the network.
Truly, the idea of sinewy fortification is exceptionally old. Press bars were utilized to strengthen workmanship in the nineteenth century, prompting the advancement of steel fortified cement. There are scriptural references to straw-strengthened earth in antiquated Egypt. The principal fiberglass vessel was made in 1942; strengthened plastics were likewise utilized as a part of flying machine and electrical segments as of now. The main boron and high quality carbon filaments were presented in mid 1960s, with utilizations of cutting edge composites to flying machine parts. The metal framework composites, for example, boron aluminum were presented in 1970. Dupont created Kevlar strands in 1973.Now composites advances and the development take placed to develop the newer metal matrix and ceramic matrix composites, as well as the carbon/carbon composites, for high temperature applications. These composite products are designed to have high mechanical performance and environmental stability with low weight.
A standout amongst the most vital strides in the use of composite materials is the creation procedure. An assortment of manufacture strategies reasonable for a few applications is accessible. They include autoclave molding, filament winding, pultruson, and resin transfer molding. This requires more stringent
and extensive quality control procedures, and skilled labors.
Fig2. Fabricated natural seed panel
Types and Classification of Composite Materials
Two phase composite materials are classified into three broad categories depending on type, geometry, and orientation of the reinforcement phase. The classification is shown in fig 3 below.
Present and future scope
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4854
area of fibers, polymers, and ceramics; requirements for high performance materials in aircraft and aerospace structure. The initial driving force I the technology development weight savings. The usage of conventional and new composite materials is intimately related to the development of fabrication methods. The assembling procedure is a standout amongst the most essential stages in controlling the properties and guaranteeing the nature of the completed item. Quality control assessment and mechanization are being presented in the assembling procedure.
Newer high volume applications, such as in the automotive industry, will expand the use of composites greatly. The energy for conservation motivates more use of lightweight materials and products.
Identification of the problem
Natural reinforced fibers are one of the examples of composite materials. Natural composite materials are made from the available materials found in nature, which are bio degradable when they are decomposed. It will not produce any harm to the environment as the plastic reinforced composite materials. The best part of natural composite material it is mostly freely available in nature and gives high strength and hardness as the metals. The fundamental point is to deliver a low weight and high quality material to the world, regardless of whether it is a characteristic composite or metal composites or glass fiber fortified or earthenware composites. Be that as it may, when it is regular composites it is more compelling as far as cost and additionally the weight.
Objective of the project
The project objectives are:
1. Experimental procedure used to fabricate a natural composite fiber.
2. To find and verify the strength and hardness of the natural composite prepared, impact and harness test performed.
3. Three different compositions are fabricated with different fiber ratios and epoxy resins respectively.
4. Comparing the composites among themselves, and also compared with the other composites. 5. Future investigation can be made on fire and
water resistance also.
Application and composition of composite materials
Why composite material?
1. Weight reduction up to 20 to 50%.
2. Single-shell shaped structures give higher quality at bring down weight.
3. High effect protection. For example, Kevlar (aramid) defensive layer shields planes have decreased coincidental harm to the motor arches that convey fuel lines and motor controls.
4. High warm steadiness
5. High harm resilience improves mishap survivability
6. Resistant to weakness/erosion
7. Structural segments made of composite materials are anything but difficult to gather. 8. Recycling utilized parts from
decommissioned flying machines is another choice accessible when utilizing aviation composites.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4855
the planes by embracing reusing of all the air ship materials made utilizing composites. 10. Although reusing of an air ship structure is a
mind boggling and costly process, it might spare cash in buying costly direct parts 11. With expanding fuel costs, business aviation
producersare under strain to upgrade the execution of flying machines, for which weight decrease is a key factor.
12. Based on the propel that is being made in composite advancement techniques, it is likely that the plane of tomorrow will be created using composite materials.
13. However, there are as yet a couple of snags to overcome before composites can supplant aluminum and other metal mixes absolutely, particularly if there ought to emerge an event of significant planes.
14. Composite innovation keeps on progressing, and the development of new sorts of composites, for example, carbon nanotubes and basalt structures will additionally quicken composite utilization.
15. However, concerning aviation, this new material won't have the capacity to totally supplant conventional metallic compounds until the point that methods are acquainted with diminish their manufacture and support costs.
Preference of Tamarind seeds and Palm Date seeds
Tamarind seed is an underutilized by result of the tamarind mash industry. Just a couple of ventures utilize the Tamarind seed, as tamarind portion powder for estimating material in the material, paper, and jute businesses. In spite of the fact that numerous
utilizations of this seed are conceivable, there have been not really some other uses for it including utilizing it as an added substance in nourishment definitions. The superb gelling cum cement attributes of decorticated seed powder can prompt a few applications in composite materials.
Chemical properties, properties of tamarind seed
Seed color: LB = Light brown and DB = Dark brown respectively each value is a mean of three determinations.
Means followed by similar superscript letters in a column are not significantly different at (P ≥ 0.05)
Table1. Proximate chemical composition of the Tamarind seed.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4856
Composition of date seeds
Table2 Date seed composition
As discussed above the project is made out of the date seeds and tamarind seeds powder. In daily use we use dates as a staple food and tamarind in daily cooking, the seeds of both dates and tamarind we usually through away as a waste product, in which the date seeds are rich high fiber, it shows high strength at extreme conditions, whereas the tamarind seed act as a natural adhesive which binds the component and gives high strength and resistance. They are corrosive resistant and fire proof. These are natural bio-degradable materials are included with feasible framework and are made into a composite material.
The mechanical properties as the intense and inexhaustible materials can be utilized to make substantial, 3-D objects with complex shapes. These seed powders can separate totally inside around two weeks subsequent to being disposed of in the earth and even discharge supplements amid its breakdown that plants can utilize. The seeds powder fiber is blended with a fortified framework to shape the polymer composite material, shabby and simple to make on vast scales and wouldn't take up arrive like plant-based bio plastics. A reasonable network is added to the date and tamarind seeds powder then the quality of the fiber increments to oppose the composite material and withstand the conditions of the earth as it is biodegradable.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4857
Araldite AW 106 / Hardener HV 953 U Key points
Araldite AW 106 / Hardener HV 953 U are a multipurpose, two components (Epoxy, Hardener), good at room temperature curing, liquid adhesive of high strength and toughness. Araldite AW 106 / Hardener HV 953 U suitable for materials like metals, ceramics, glass, rubber, plastics and most other materials in common use. It is a good adhesive for the craftsman as well as most industrial applications.
Table3 specification of epoxy resin
Pretreatment: If the strength and durability of a bonded joint depends on what kind of treatment on the surface is done before bonding. At least, joint surfaces should be cleaned with a good DE-greasing agent such as acetone, iso-propanol (for plastics) or other DE-greasing agents in order to remove all traces of oil, grease and dirt. Low grade alcohol,
gasoline (petrol) or paint thinners should never be used, because it reacts quickly and can be harmful. The strongest and most long-lasting joints are obtained by either mechanically abrading or chemically etching the DE-greased surfaces.
Application of adhesive
The resin/hardener blend might be connected physically or by utilizing robot to the dry joint surfaces. A layer of glue 0.06 to 0.12 mm thick will ordinarily confer the best lap shear quality to the joint. The joint parts ought to be set and dried in a settled position when the glue has been connected.
Mixing ratios of Epoxy and Hardener
The best case is a 1/1 ratio with even viscosity, worst case is a 10/1 ratio with a wide viscosity difference. It also depends on the type of epoxy resin/Hardener used. The type of cartridge can also have a dramatic effect on dispense quality, especially when used in a pulsing mode. Larger and thin walled cartridges can induce a lead/lag effect where resin/hardener show an extreme ratio change in a very short period due to the expansion and relaxation of the cartridge barrel. The thicker walled cartridges show much less tendency to produce this lead/lag effect which is a primary cause on intermittent tacky on small, Potting or casting.
Table4 mixing ratio of epoxy resin
Appearance and odor: Clear slight yellow, slightly viscous liquid with a slight ammonia-like odor Solubility in water: slight.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4858
The date seeds were separated from their fruits manually or mechanically, thereafter washed and cleaned to remove contaminants and they were dried and grinded with hammer mill to obtain filler powder. The filler powder were made to pass through wire mesh screen to obtain a fine particle size, thereafter oven dried at temperature of about 60⁰C before the use so as to reduce the moisture content. Samples were thereafter stored in desiccators.
Fig4. Seeds of Date Palms
Fig5.Date seeds powder
The Tamarind seeds were separated from their Tamarind pulp, thereafter washed cleaned to remove contaminants and they were dried and roasted at 90⁰C and grinded with hammer mill to obtain filler powder. It is then filtered to fine particles, thereafter oven dried for some time to reduce the moisture content. Samples were thereafter stored in desiccators.
Fig6. Tamarind and tamarind seeds
Fig7. Tamarind seeds powder
Reinforcement that is used in the composite material is this completely dried powder which is mixed with the matrix suggested possessing the particulate reinforced matrix. This seeds powder will have good strength when compared to other biodegradable materials.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4859
Fig8. Epoxy resin Araldite AW106, hardener HV959
At the point when hand blending the epoxy pitches and the hardeners, it is best to empty the tar into the blending vessel first in a compartment. The pitch and hardener are included the proportions and blended in the compartment for a period until the point that we get a decent vertex amidst the arrangement in the holder. At the point when a decent vertex is gotten in the arrangement then the seeds powder is added to the vertex of the framework in the holder. The powder blended into the network is mixed utilizing a mix stick physically or by utilizing mechanical machine until the point when it frames a decent blend. It doesn't require any temperature or heat. The blend ought to be blended with no air pockets and it must be perfect and free from clean also. It should make a uniform conveyance all through the synthesis by scratching the sides and base of blending vessel every now and again.
Fig9. Mixing of epoxy resin and hardener
After the items have been blended altogether, the blend ought to be filled the shape or utilized as a part of the cement step. Regularly, the final result must be absolutely free of voids and air pockets. The readied composite material is filled the form of the required shape. The state of the form is secured out as a composite material. This ought to be done in various proportions of the powders. Utilizing these strategy three test examples is manufactured, utilizing the
accompanying proportions appear in the accompanying tables.
Table5 specimen 1
Table6 Specimen 2
Table7 specimen 3
The mould is dried for 24 hours and rested in the room temperature. After it dries take out the natural composite panels. The composite panels procured out are hard and high in strength. Fig 10 shows the after curing process of the natural composites mixture of tamarind and date seed powders along with epoxy resin.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4860
Testing Impact testing
In real work on, building segments amid the examination are constantly subjected to different sorts of burdens specifically static and dynamic burdens. Dynamic burdens are recognized by high rate of alter in stack size and course. Invert occurs if there should be an occurrence of static burdens. In the hardness test and malleable tests, stack is expanded gradually that relates to the conduct of material under pretty much static stacking condition. Wide range rate of stacking can be utilized as a part of tractable test. Rate of stacking drives the strain rate thus rate of solidifying which can influence mechanical conduct of material.
The toughness test simulates service conditions often encountered by components of the system used in transportation, agricultural, and construction equipment. A material high effect protection is said to be an intense material. Strength is the capacity of a material to oppose both crack and twisting. Sturdiness is the mix of quality and malleability. To be intense a material must displays both genuinely great quality and malleability to oppose splitting and misshappening under effect stacking. Indents are had purposefully in effect test examples to expand the stress concentration in order to build inclination to break as the majority of the mechanical segments have stretch raisers. To withstand an effect compel, a scored material must be extreme.
Fig11.Principle diagram of toughness test
To study the behavior of material under dynamic load conditions toughness test is frequently conducted. There are two methods used for toughness testing namely Izod and Charpy test, based on common principle applying the load at high rate and measuring the amount of energy absorbed (kgm. or joule) in breaking the sample due to impact. However, there are some differences also in these methods in terms of sample size and shape, method of holding of the sample and maximum energy content of pendulum that hits the sample during the test.
Table8showing types of impact tests
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4861
Fig12. Standard specimen for Charpy test
Results of impact tests are conveyed in terms of either amount of energy absorbed (Nm) or amount of energy absorbed per unit across sectional area (Nm/cm2) by standard sample. These tests are useful for comparing the resistance to impact loading of different materials or the same material in different processing conditions such as heat treatment, procedure and mechanical working etc. Resistance to the impact loading of a material appreciably depends on the surrounding temperature. Therefore, temperature toughness test is conducted must me reported with results.
Fig13. Schematic diagram showing influence of test temperature on toughness
For Charpy v-notch test I used the ASTM D-256 test procedure, and the equipment used is:
Krystal Elemec. Model no: KI300. S.no: 98/1081. Range -168J for Izod.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4862
Fig 15. Before impact testing specimens A ,B,C.
Fig16.Specimens B, C, A shown after impact testing.
Rockwell Hardness Test
The fig.18 demonstrates the Rockwell shore hardness analyzer. The Rockwell hardness test strategy comprises of indenting the test material with a jewel cone or steel ball indenter. The indenter is constrained into the test material under beginning minor load F0 (Fig.18 A) as a rule 10 kgf. At the point when balance has been achieved, a demonstrating gadget, which takes after the developments of the indenter reacts to changes top to bottom of entrance of the indenter, is set to a datum position. While the underlying minor load is as yet connected an extra real load is connected with coming about increment in infiltration (Fig 18. B). at the point when adjust has again achieved, the extra real load is expelled yet the underlying minor load is as yet kept up. Evacuation of the extra significant load permits an incomplete recuperation, so diminishing the profundity of infiltration (Fig 18. C).
the changeless bring up inside and out of entrance, is utilized to process the Rockwell hardness number.
Fig17. Shore hardness tester
Fig18. Rockwell Principle
HR = E – e
F0= preliminary minor load in kgf F1= additional major load in kgf F= total load in kgf
e= permanent increase in depth of penetration due to major load F1 measured in units of0.002 mm
E= a constant depending on form of indenter: 100 units for diamond indenter, 130 units for steel ball indenter
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4863
Here for hardness testing I have used the ASTM D 2240:2003 test procedure to test the specimens, and the equipment used is:
SHORE HARDNESS TESTER.
Model no: SHR-GOLD. S.no: 17773.
Standard Block: 50 Shore D
Test reports after testing in laboratory are
Results and Conclusion Results
Specimens are taken as per the proportions shown in fig.19 by showing the variations in epoxy resin quantity as well as the tamarind and date seed powders. The specimens A, B, C is made with the powders of different compositions. Each specimen weight approx. 140 Gms and dimensions are 15MM THK X 130MM LG.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4864
Charpy impact tests are performed on each specimen for three trails as per ASTM D-256 on range- 168J for Izod capacity KRISTAL ELMEC equipment. Each specimen is machined as per standard dimensions need and a V-notch is made on three test pieces of each specimen A,B,C. The results obtained are shown in fig.20for each specimen the impact result obtained is slightly different and maximum on specimen C is observed.
Table9 observed values impact test
Shore Hardness test is also performed as per standard ASTM D-2240 on SHR-GOLD equipment and the standard block is 50 SSHORE D. the three specimens are taken each for three trail test pieces and the hardness test is done using intender D. The results obtained varied on comparing each other. The specimen C with equal quantity of tamarind and date seed powders showed greater hardness compared to other two specimens A and B, which shown in fig 20.
Table10observed values of hardness test
Fig20. Shore hardness test, Avg. Hardness VS Specimen
An observational experiment is also experimented by placing the above composite in water for 48 hours and it is observed that there is a not much absorbance of the water by the composite; minute moisture can be seen on the internal structure of the composite. This shows that this composite material there is an advantage of using this as water proofing material where it can be treated as roofing material, internal automobile accessories and many other various uses can be found.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4865
increase in the weight (i.e. 0.1%). This shows the fabricated composite is a slow absorbent of water. But compared to the other composites it shows better results. From the above results the above prepared, composite can be used as the as false roofing instead of the thermocol and Plaster of Paris.
The above natural composite prepared can also bear the fire while the thermocol cannot withstand under fire conditions. The tamarind and date seed powder composite can be a best replacement for termocol, Plaster of Paris and it give a grandeur look to the sealing. The fig. 21 shows how we can use the composite as the false roofing. Further testing of the above composite material in various aspects, such as automobile industries, construction industries, it can be of great use in the market in various fields.
Fig21. Showing the example of false roofing
Much more research can be done using different combinations to increase the strength and hardness of materials. Due to great need of composite materials in various fields in order to cut off cost and weight, quality of the materials plays major role in replacing existing range of materials, and also it can be tested in the automobile industries. Furthermore investigation can be done on the fire proof and the water absorption of the composite.
Engineering-mechanics-of-composite-materials-Isaac M-Daniel-o-isha 1994. Oxford university press.
 Processing and characterization of Epoxy composites reinforced with short Palmyra fibers by somenbiswal NIT Rurkela 2016.
 Hull D, 1981, an Introduction to Composite Materials, (Cambridge University Press)  Mechanics of composite materials Autar k.
Kaw 2006 by Tailor and Francis Group.  Mechanics of composite materials Robert M.
 Epoxy Resins, Curing Agents, Compounds, and Modifiers: An Industrial Guide, By Ernest W. Flick
 T.-M. Wu and C.-Y. Wu, Biodegradable poly (lactic acid)/chitosan-modified montmorilloniteNano composites: preparation and characterization, Polymer. Degrade. Stab.
91, pp. 2198–2204, 2006.
doi:10.1016/j.polymdegradstab.2006.01.004.  El- Siddig, K, Ebert G, Liidders (1999)
Tamarind (TamarindusIndica) A Reviewon multipurpose tree with promising future in the Sudan. J. Applied Botany 73:202-205.
 Joye DD, Luzio GA (2000) Process for selective extractionofpectinsfrom plant material by differentialph. Carbohydrate Polymer 43: 337-342.
Ghose TP, Kishna S (1942) Decortications of tamarind seed. J.IndianChem.Soc. Ind. And News Ed5: 114.
Available online: https://edupediapublications.org/journals/index.php/IJR/ P a g e | 4866
Bhattacharya S, Bal S, Mukherjee RK, Bhattacharya S (1993) some physicaland engineering properties of tamarind (TamarindusIndica) seed. J Food Eng.18: 77-89.
H. Ehrlich and H. Worch, "Sponges as natural composites: from biomimetic potential to development of new biomaterials," in Porifera Research: Biodiversity, Innovation &Sustainability, University of Technology, Germany, 2007.
Jimenez, L., Sibaja, M., Alvarado, P., Vega, J., Jimenez, G., Barreiro, M.F., Cateto, C.A., and Lopretti, M., “Rigid Composite Materials from Olive Brush Seed and Unsaturated Polyester Resin", ANTEC, (2008).